**50th Anniversary of JTAM**

**TEMPERATURE INCREASE ASSOCIATED WITH PLASTIC**
**DEFORMATION UNDER DYNAMIC COMPRESSION:**

**APPLICATION TO ALUMINIUM ALLOY AL 6082**

Jos´e-Luis P´erez-Castellanos

*University Carlos III of Madrid, Department of Continuum Mechanics and Structural Analysis,*
*Madrid, Spain; e-mail: percaste@ing.uc3m.es*

Alexis Rusinek

*National Engineering School of Metz (ENIM), Laboratory of Mechanics, Biomechanics, Polymers*
*and Structures (LaBPS), Metz, France; e-mail: rusinek@enim.fr*

The temperature increase associated with plastic deformation of a ma-terial under loading may be measured using several techniques such as infrared thermography (IRT). The present work investigates the tem-perature increase at diﬀerent high strain rates and initial test tempe-ratures, using an aluminium alloy Al 6082. A Split Hopkinson Pressure Bar (SHPB) was applied to induce high strain rates to the material and an infrared camera was used to measure the temperature increase. Nu-merical simulations of dynamic tests were performed to calculate the temperature increase and to gain a better understanding of the process by local measurements. Thus, a detailed ﬁnite-elements model was deve-loped to simulate the dynamic compression test. The fraction of plastic work converted into heat was estimated using the Zehnder model. Nu-merical results in terms of the strain rate and initial temperature eﬀect on the material temperature increase are reported and compared with experiments.

*Key words:*infrared thermography, plastic strain, adiabatic heating,
Hop-kinson bar

**1.** **Introduction**

Mechanical energy produced during plastic and elastic deformation of a metal
is partially converted into heat while the rest is stored as deformation energy
*(Hodowany et al., 1999; Kappor and Nemat-Nasser, 1998). This stored energy*
remains in the material after loading as internal defects, phase changes and

other permanent microstructural changes. The heat generated, proportional to a part of the mechanical work, induces a temperature increase of the material. The thermal-balance equation for a visco-plastic isotropic material is given by Eq. (1.1). It does not consider the eﬀect related to phase-transformation processes in the heat generation as discussed in Rusinek and Klepaczko (2009)

*λ∇*2*T − ˙T = −* *β*
*ρCP*
* σ: ˙εp*+

*α*

*ρCP*

*E*

*1 − 2v*

**T tr ( ˙ε***e*

_{)}

_{(1.1)}

*where λ is the thermal diﬀusivity of the material, T is the absolute *
*tempera-ture, β is the Quinney-Taylor coeﬃcient (Taylor and Quinney, 1934), *
*(propor-tion of plastic-deforma(propor-tion energy converted into heat), ρ is the mass density,*

*CP* * is the speciﬁc heat, σ is the stress tensor, ˙εp* is the plastic strain-rate

**ten-sor, ˙ε**e*is the elastic-strain-rate tensor, α is the thermal-expansion coeﬃcient,*

*ν is Poisson’s ratio, and E is Young’s modulus.*

Close to 10 s*−1* _{for metals (Klepaczko et al., 2009; Oussouaddi and }*Kle-paczko, 1991; Rusinek and KleKle-paczko, 2001; Rusinek et al., 2007) no heat is*
exchanged with the surroundings, and adiabatic conditions may be assumed

*λ∇*2_{T = 0. If thermoeslasticity is not considered, then the temperature }*incre-ase ∆T , may be calculated as a function of the plastic strain εp*

*∆T (εp*) =
*εp*
*max*
Z
0
*β*
*ρCP*
*σ(εp) dεp* (1.2)

*where σ is the equivalent stress under uniaxial deformation and εp* is the
corresponding equivalent plastic strain.

*It is usual to consider β as constant in such calculations. Nevertheless, it*
*is accepted that β depends on the plastic strain. Diﬀerent models (Aravas et*

*al., 1990; Rosakis et al., 2000; Zehnder, 1991) to deﬁne the Quinney-Taylor*
*coeﬃcient β, have been developed. Based on the Zehnder model, related to the*
calculation of stored energy by unit of dislocation density, the Quinney-Taylor
*coeﬃcient β, may be deﬁned as below*

*β(εp) ≈ 1 −∂σ(ε*
*p*_{)}
*∂εp*
1
*E*
*˙εp*
(1.3)

*where E is material Young’s modulus.*

If a potential hardening law is used (which allows an isotropic behaviour to be deﬁned while considering just hardening), an analytical expression for the

*Quinney-Taylor coeﬃcient β(εp*), Eq. (1.4), may be deﬁned (Zehnder, 1991)
from Eq. (1.3)
*β(εp) = 1 − n**ε*
*p*
*ε*0
*n−1*
(1.4)
*where ε*0 *is the yield strain and n is the hardening exponent of the material.*
The temperature increase in a specimen deformed during plastic deformation
may be calculated using Eq. (1.2) and Eq. (1.4).

There are at least two procedures for measuring the temperature
*incre-ase ∆T associated with the plastic strain εp*_{. The ﬁrst one is based on the}
use of a rapid-response thermocouple connected to the specimen tested. The
second one is based on the measurement of the thermal radiation of the
spe-cimen emitted during deformation. It corresponds to the temperature ﬁeld
observed on the surface of the material.

The IRT technique has been widely used to correlate plastic strain to
*temperature increase ∆T (εp*_{) in metal and polymeric materials. This }
techni-que is steadily more used due to the development of new high-speed infrared
cameras. During the last decade, several authors were using the IRT
tech-nique to estimate the temperature increase of materials during elastic and
plastic deformation. For example, Kappor and Nemat-Nasser (1998),
*Man-son et al. (1994), Rabin and Rittel (2000) measured the temperature *
incre-ase under dynamic compression tests using a SHPB device. Chrysochoos and
Louche (2000) applied thermographic analysis to the deformation process of
*Polymethyl-methacrylate (PMMA). Trojanowski et al. (1998) used IRT to *
in-vestigate the heat generation in an epoxy resin and in metal specimens, coupled
to a SHPB. Titanium-alloy specimens were tested by Macdougall and Harding
(1998), using a split Hopkinson torsion and tensile bars and by using an
in-frared radiometer to measure the temperature increase during the test. The
IRT technique to investigate impact processes of steels at high strain rates was
*used by Guduru et al. (2001), Rusinek et al. (2003), and Rodr´ıguez-Mart´ınez*

*et al*. (2010).

The objective of the present study is to investigate the temperature
*in-crease ∆T associated with the plastic strain εp* _{at high strain rates ˙ε}p_{using}
an aluminium alloy Al 6082. The technique used to measure the temperature
increase is based on the IRT. Concerning the mechanical loading, a SHPB
is used to reach high strain rates under dynamic compression. Coupling the
*SHPB and IRT technique, it allows the temperature increase ∆T to be deﬁned*
*and estimated at high strain rates during plastic deformation ∆T (εp _{, ˙ε}p*

_{).}

For the test simulation, a detailed numerical model of the SHPB test was developed using a FE code. With this 3D model, extensive numerical analyses were made to calculate the temperature increase and other local quantities to

compare with the experiments. This kind of technique using coupling
experi-ments and simulations, steadily more used, is called the “Inverse Method”. It
allows one to reach local quantities to complement measurements of
macro-scopic behaviour made during experiments, for a better understanding of the
*material behaviour (Rusinek et al., 2008; Migu´elez et al., 2009).*

**2.** **Test description**

Guzm´*an et al. (2009), and P´erez-Castellanos et al. (2010) have developed an*
original set-up and a SHPB testing procedure with a simultaneous
*measure-ment of the temperature increase ∆T (εp _{, ˙ε}p*

_{), using an infrared camera (IRC)}

*and the dynamic mechanical behaviour of the material σ(εp, ˙εp, T ). The next*

part of the paper provides a detailed description of the technique used.

**2.1.** **Test set-up**

For dynamic testing, a SHPB was used. This device, developed originally by
Kolsky (1949) consists of two coaxial bars between which the specimen is ﬁxed.
A cylindrical striker of the same material and with the same cross-sectional
area as the bars is launched, using a pneumatic gas gun, to impact against
the incident bar. As a result of the impact, a compressive square-shaped pulse
travels through the incident bar until it reaches the specimen; the magnitude
*of the incident wave is σi* *= ρCV*0*/2 with a duration of tp* *= 2Lp/C. In the*
*previous formulas, ρ is the bar density of the material; C is the elastic wave*
*speed, which depends on Young’s modulus E; with C =* p

*E/ρ; V*0 is the
*velocity of the striker just before impact, and Lp* is the striker length. When
*the incident wave εi*reaches the incident bar-specimen interface, it is split into
*reﬂected εr, and transmitted waves εt*. Two strain gauges, on full bridge, ﬁxed
on the incident bar and the transmitter bar, respectively, allow recording of
the elastic strain waves. The strains are related to the stress quantities using
Hooke’s law.

The temperature increase during the test is measured using an IRC with
a temperature resolution of 20 mK. The frequency acquisition of the camera
may be increased by reducing the frame size (subwindow mode). A subwindow
of 64x16 pixels was used, thus achieving 3290 frames per second, with an
*acquisition time of 40 µs (TACQ*). Before starting the tests, the camera was
calibrated using a black body from 273 K to 373 K.

The specimen is placed in a test chamber to isolate it from spurious external radiation. Thus the IRC measures only thermal radiation. Inside the chamber, there are electrical resistances controlled by thermocouples with which the specimen may be heated until reaching the deﬁned test temperature. The maximum temperature allowable is 573 K.

A dark chamber is placed between the test chamber and the IRC. This chamber was designed taking into account the working focal distance of the IRC.

Figure 1a shows a picture of the test chamber and the dark chamber con-nected to the Hopkinson bar. Figure 1b shows a picture inside the test chamber with the electrical resistances to enable the test to be performed at diﬀerent initial temperatures.

Fig. 1. (a) Coupled SHPB, test chamber, and dark chamber, (b) internal test-chamber description

A fundamental aspect of the testing system is the synchronism between the SHPB and the IRC. This synchronism is achieved by means of a trigger system. The synchronization system consists of two photoelectric sensors, two optical ﬁbres, and a time counter. During experiments, the photo-sensors detect the striker arrival and generate a trigger signal. By the use of this synchronization system, it is possible to associate the temperature measured by the IRC with a value of the strain in the specimen during the deformation process.

**2.2.** **Test procedure**

The test procedure is based on the classical SHPB testing methodology. The main diﬀerence is that several mechanical and electronic time intervals must be controlled to ensure synchronism between the SHPB and the IRC, allowing a better analysis on time of the signals.

*The strain rate ˙ε imposed on the specimen depends on the striker *
*veloci-ty V*0and is proportional to the air pressure stored in the gas gun chamber and
*to the specimen length Lo. The nominal strain εN, the strain rate ˙εN*, and the
*nominal stress σN*, imposed on the material may be calculated with knowledge
*of the incident wave εi, the reﬂected wave εr, and the transmitted wave εt*,
recorded, using the following expressions, Eq. (2.1). This is based on the
the-ory of one-dimensional elastic-wave analysis while assuming mechanical-force
equilibrium of the specimen

*εN(t) =*
*2C*
*Lo*
*t*
Z
0
*εr(τ ) dτ* *˙εN(t) =*
*2C*
*Lo*
*εr(t)*
*σN(t) = E*
*A*
*AS*
*εt(t)*
(2.1)

*where C is the velocity of the elastic waves, AS* is the initial cross section
*of the specimen, A is the cross section of the bar, Lo* is the initial length
*of the specimen, and E is the Young modulus of the bar material. The true*
*stress σ, and true strain ε, may be calculated, respectively, using the following*
*expressions, Eq. (2.2), and assuming plasticity with constant volume ν = 0.5*

* σ = σ(1 − εN*)

*ε = − ln(1 − εN*) (2.2) The physical process of temperature measurement by the IRC is described as follows. The IRC receives and measures the outcoming radiance from the

*object Rout. This radiance has two components: the emitted Remi*, and the

*reﬂected Rref. The emitted radiance may be calculated as Remi*

*= ǫR*0

*(Temi*)

*where R*0

*(Temi*) is the radiance emitted by the black body for the same

*spe-cimen temperature Temi, and ǫ is the specimen-surface emissivity factor. The*

*reﬂected radiance may be calculated as Rref*

*= rR*0

*(Tamb) where R*0

*(Tamb*) is

*the radiance emitted by the black body at room temperature Tamb, and r the*

*specimen-surface reﬂectance (r = 1 − ǫ). The radiance received and measured*by the IRC is related to its emitted and reﬂected components as

*Rout* *= ǫR*0*(Temi) + (1 − ǫ)R*0*(Tamb*) (2.3)

*Rout* *is measured using the IRC, R*0*(Tamb*) may be calculated using the
*well-known Plank’s law expression, and ǫ must be ﬁrstly estimated. From these*
*parameters, R*0*(Temi*) may be calculated using Eq. (2.3). Finally, the
*tempe-rature of the specimen T may be deduced as the value at which the integral*
*of the Plank law expression R*0*(λ, T ), over the spectral range of the camera,*
*equals to R*0*(Temi*).

*The IRC records the radiation during an exposure interval [tFR, tFR* +

*TACQ] where tFRis the time when the frame recording starts and TACQ* is the
acquisition time. From the recorded radiation, a temperature value is
*determi-ned. This temperature is associated with the middle point, tFR+ TACQ/2, of*
the exposure interval to relate it with the plastic strain, using the synchronism
system.

In each test, a set of successive IR images was also recorded by the IRC. The
images were processed to draw a temperature map and a temperature proﬁle
*along a generatrix line (∆T vs. pixel). This temperature proﬁle includes the*
specimen and one segment of each bar (incident and transmitter) on both sides
of the specimen with a total length equal to the horizontal dimension of the
*window used (64 × 16 pixels), Fig. 1b and Fig. 3.*

The frame rate of the camera used does not allow more than two or three temperature measurements during the complete loading time. Therefore, to have more values of the temperature increase, several tests must be perfor-med for the same initial conditions. Thus, the temperature-increase value

*∆T (εp _{, ˙ε}p*

_{) for a set of initial conditions, was calculated using an average }

*qu-antity ∆T = N−1*P

*N*

1 *∆Ttest* *where N is the number of tests performed.*

**3.** **Results and discussion**

**3.1.** **Material**

The material used in this study is an aluminium alloy Al 6082
*(Mrówka-Nowotnik and Sieniawski, 2005; Mann et al., 2007; Manping et al., 2008; Agena,*
*2009; Dadbakhsh et al., 2010). This alloy is a medium-strength structural alloy*
that includes in its chemical composition 0.7-1.3 Si, 0.4-1.0 Mn, 0.6-1.2 Mg and
0.4-0.15 Cr; the manganese controls the grain structure and size. Depending
of the manganese added, this alloy has high values of mechanical properties
and is used for industrial application where both lightness and high strength
are required. In Table 1, the mechanical static parameters characterizing our
alloy Al 6082 are reported.

**Table 1. Mechanical parameters of alloy Al 6082**

Tensile strength Yield stress Elongation Young’s modulus

[MPa] [MPa] [%] [GPa]

300-320 280 13 69.5

The material was supplied in the form of extruded bars and machined to the ﬁnal geometry: 7.0 mm long and 14 mm in diameter inducing a ratio

*s*0 *= h*0*/d*0*= 0.5. The specimens previously underwent a process of polishing*
and a lubricant (MoS2*) was used to reduce the friction eﬀect µ between the*
*specimen and the bars. The friction eﬀect is related to the parameter s*0 as
*reported in Malinowski and Klepaczko (1986), and Jankowiak et al. (2011). All*
the specimens before the tests were covered with soot to increase the
*material-emissivity factor ǫ.*

*The value of the material-emissivity factor ǫ was calculated *
experimen-tally. A specimen was heated on the heating plate from room temperature to
393 K. During the heating process, the temperature time course was measured
simultaneously by the IRC and by a thermocouple ﬁxed on the specimen. The
two temperature measurements were compared to determine the
*emissivity-factor value ǫ of the material considered. With the use of this technique, the*
*average of the emissivity factor was estimated to ǫ = 0.8.*

**3.2.** **Experimental results**

Several compression tests were performed at room temperature, 293 K, for
diﬀerent strain rates. The reproducibility of the tests was veriﬁed by comparing
several results under the same experimental conditions. Thus the results in
*terms of σ −εp _{and ∆T −ε}p*

_{curves for the same set of experimental conditions}were consistent with a maximum diﬀerence of 1% for an imposed condition in terms of the strain rate and initial temperature.

Figure 2 shows, as an example, the true stress/true plastic-strain
relation-ship that resulted at room temperature and diﬀerent strain rates varying from
300 s*−1* _{¬ ˙ε}p_{¬ 1500 s}−1_{.}

From the true-stress/true-strain curves, the logarithmic
*strain-rate-sensitivity coeﬃcient was calculated, m = (∂ log σ/∂ log ˙ε)|ε,T* *= 0.03, which*
may be considered as a moderate value in the interval of the strain rates
te-sted. Nevertheless, remarkable temperature sensitivity of this alloy is noted,

*ν = (∂ log σ/∂ log T )|ε, ˙ε= −0.4.*

Figure 3 shows, as an example, several proﬁles of temperature increase that
*resulted during the tests at room temperature for a strain rate of ˙ε = 600 s−1*_{.}
Each proﬁle shows a relatively constant temperature value with two peaks
corresponding to the perimeter of the circular bases of the specimens. These
peaks are due to the friction eﬀect inducing an additional temperature increase
and, therefore, not considered to represent the temperature increases in the
specimen.

Table 2 presents the results of the measured temperature increase including
*the initial temperature T*0 *the average strain rate reached during the test ˙ε*

*p*
,

*Fig. 2. σ − εp* _{curves for Al 6082 alloy at room temperature; (a) ˙ε}p_{= 300 s}*−1*,

*(b) ˙εp*= 600 s*−1, (c) ˙εp*= 1000 s*−1* *and (d) ˙εp*= 1500 s*−1*

Fig. 3. Proﬁles of temperature increase corresponding to diﬀerent strain levels at
*room temperature and strain rate ˙εp*= 600 s*−1; (a) εp= 0.027 and (b) εp= 0.046*

*the plastic strain level εp*_{, and the associated recorded temperature increase}
*under dynamic compression ∆T .*

*From the previous values, Table 2, it is observed that ∆T (εp*_{) did not}
depend on the strain rate for an imposed strain level and initial temperature;
this is due to a reduced strain-rate sensitivity of the alloy Al 6082, as discussed
previously.

* Table 2. Tests results: test temperature T*0

*, plastic strain rate reached ˙ε*

*p*

,
*plastic strain εp* _{and the associated temperature increment ∆T}

*T*0 [K] *˙ε*
*p*
[s*−1*_{]} _{ε}p_{[–]} * _{∆T [K]}*
600 0.014 1.4
296 600 0.027 3.0
600 0.046 5.8
296
1000 0.026 3.1
1000 0.047 6.1
1000 0.07 9.7
1000 0.092 13
1500 0.038 3.5
373 1500 0.127 15
1500 0.195 20

Immediately after the process of plastic deformation ended, a small
tem-perature decrease was detected. This temtem-perature decrease was due to the
elastic recovery as observed precisely under a quasi-static compression test.
The load applied to the specimen consisted of a periodic compression force
with an amplitude of 32.3 kN and a frequency of 0.185 Hz. This load
*amplitu-de corresponds to a material-stress level of σloading* = 210 MPa, which is less
than the material yield stress. The frequency value was chosen to be able to
reproduce it on the test machine.

Figure 4 shows the loading force vs. time and the temperature increase vs. time relations.

Fig. 4. Loading force vs. time and temperature vs. time relations measured during the experiment

The maximum temperature increase was found to be close to 0.5 K. It
was also observed that the decreasing slope deﬁnes a temperature decrease
of the same magnitude as the thermal expansion parameter of the material.
*The temperature increase, ∆T (εp, ˙εp*), corresponds to a rate of 0.42 K/s. This
rate corresponds exactly to the rate calculated using the analytical expression
derived by Thomson (1853), which is the last term of Eq. (1.1) and representing
the temperature variation associated with the elastic strain, Eq. (3.1).

The temperature increase, as elastic recovery, proved to be of the same order of magnitude, close 0.5 K. Thus, the temperature decrease observed at the end of the test may be considered to correspond to the elastic recovery process.

**3.3.** **Numerical analyses**

A three-dimensional ﬁnite-element model was used to simulate the SHPB tests. The commercial ﬁnite-element code ABAQUS/Explicit, 2006, was used to investigate the precise thermo-mechanical process in the specimen under dynamic loading and the phenomenon of elastic-wave propagation. The FEM model developed is described in the following sections.

*3.3.1.* *Model description*

The model includes the two elastic bars, the striker, and the specimen using real dimensions (incident and transmitter bars 1 m long with a diameter of 22 mm and for the striker a length of 330 mm with the same bar diameter; Fig. 5.

Fig. 5. 3D ﬁnite element model of SHPB test

The specimen and bars are free of movement along the bars axis. The radial movement of the nodes on the model axis is restricted.

The mesh of the incident bar, the transmitter bar, the specimen, and the striker were made using hexahedral elements with 8 nodes, C3D8R (ABAQUS/Explicit, 2006), reproducing the total geometry of the device. The

density of the mesh directly inﬂuences two fundamental factors of the analysis: the accuracy of the solution reached and the time of calculations. Therefore, it is necessary to achieve a balance between these two variables. The study of the sensitivity of the mesh was carried out before beginning the numerical analyses considering just the incident and the transmitter bars.

Several numerical models with FE meshes with 18 320 to 34 508 elements
*were considered. On the ﬁrst time, a comparison was made of the incident εi*,
*the reﬂected εr, and the transmitted εt* waves calculated using these
diﬀe-rent numerical models. It was found that there is no strong variation between
the wave proﬁles and level calculated (Fig. 6). On the second time, the
tem-perature increase on the specimen surface calculated using these numerical
models were also compared; as a result, minor inﬂuence of the mesh density
on the temperature increase (in the interval of elements number considered)
was deduced. Thus, the density of 18 320 elements was considered optimal.

Fig. 6. Analysis of the mesh-sensitivity of the SHPB model using only the transmitter bar

The contact conditions between the surfaces of the striker-incident bar, incident-bar specimen, and specimen-transmitter bar were taken into account. The tangential interaction between the contact surfaces can be established by means of Coulomb’s friction law.

Based on the Klepaczko and Malinowski model (Malinowski and Klepacz-ko, 1986), additional energy for a deformation range is observed depending on the specimen ratio used during the tests. This energy, related to friction, in-duces an extra stress increase; the stress level will change, increasing with the friction coeﬃcient. Thus, the stress level measured includes material behaviour and friction eﬀects. To correct the latter, the model proposes the expression

*µ(ε) =* *σ − σ*0

*σ* *3s*0*[exp(ε)]*
3

*where σ is the compressive true stress, σ*0is the compressive true stress
*deter-mined for an ideal test without friction specimen/bars, s*0 *= h*0*/d*0 is the ratio
*between the initial specimen height and diameter, and ε is the true strain.*

The Klepaczko and Malinowski model has some limits and may be used as
*an average range of µ varying from 0 to 0.25. A recent complete analysis of*
*this model is reported in Jankowiak et al. (2011).*

*An experimental characterization of the friction coeﬃcient µ(ε) was carried*
out using the Klepaczko and Malinowski model. Figures 7a and 7b show the
*relation between µ and ε calculated for a strain rate of 300 s−1* _{and 600 s}*−1*_{,}
*respectively. It can be seen that µ remains more or less constant and equal*
to 0.09. This value of friction coeﬃcient was the one used during numerical
calculations (the same for all test conditions) and implies no contact.

*Fig. 7. Relations µ − ε for diﬀerent strain rates under dynamic compression,*
Eq. (3.1)

*During the experiments, the striker velocity V*0 just before impact, was
me-asured with two ﬁbre-optic photoelectric sensors. This velocity was used during
numerical simulations as the initial boundary condition. The wave
transmis-sion through the bars occurs after the impact, and the incident, reﬂected, and
transmitted waves can be calculated along the mesh, and more precisely, for a
distance corresponding to it where the strain gauges are glued along the bars.
The material of the incident and transmitter bars is an Inconel steel:
Young’s modulus equal to 211 GPa and Poisson’s ratio equal to 0.3; the density
considered is equal to 8190 kg/m3_{. The material of the striker is steel: Young’s}
modulus equal to 207 GPa and Poisson’s ratio of 0.3; the density considered is
7800 kg/m3_{.}

*To describe behaviour of the isotropic alloy Al 6082, the J*2 theory was
assumed to deﬁne the ﬂow stress. The elastic constants were deﬁned from
the corresponding experimental test. The hardening function considered was

deﬁned using the Johnson-Cook model, Eq. (3.2), since the material exhibits
a low strain-rate dependency (frequently reported for aluminium 6082). This
model is well deﬁned to describe this kind of material behaviour (linear strain
rate sensitivity)
*σ(εp, ˙εp, T ) = [A + B(εp*)*n*]*1 + C ln* *˙ε*
*p*
*˙ε*0
*(1 − T∗m*_{)} _{→}*˙εp _{ ˙ε}*
0

*σ(εp, T ) = [A + B(εp*)

*n](1 − T∗m*

_{)}

_{→}*˙εp*

*0 (3.2) with*

_{< ˙ε}*T∗*

_{=}

*T − Troom*

*Tmelt− Troom*

*where σ is the equivalent stress, εp* _{is the equivalent plastic strain, ˙ε}p_{is}
*the equivalent plastic strain rate, ˙ε*0 *is the reference strain rate, Tmelt* is the
*melting temperature, and Troom* is the room temperature. As material
*para-meters, A is the initial yield stress, B is the hardening modulus, n is the*
*hardening exponent, C is the coeﬃcient of strain rate sensitivity, and m is*
the temperature sensitivity exponent.

*The parameters A, B, C, n, and m were calculated by applying the *
root-mean-square method coupled to Eq. (3.2) and based on experimental true
*stress/plastic strain curves obtained at 296 K for ˙εp* = 300 s*−1*_{, at 296 K for}
*˙εp* = 1000 s*−1 _{and at 373 K for ˙ε}p*

_{= 1500 s}

*−1*

_{. Figure 8 shows the experimental}

*true stress/plastic strain curve obtained at 296 K for ˙εp*= 600 s

*−1*

_{and the}corresponding true stress/plastic strain curve using the values calculated for

*parameters A, B, C, n, and m. A good agreement was found between the*experiments and numerical results.

*Fig. 8. Experimental and J − C true stress-plastic strain curves for a test at 296 K*
*and ˙εp*

= 600 s*−1*

*Non-constant values of the Quinney-Taylor coeﬃcient β were considered.*
The previous relation proposed by Zehnder, Eq. (1.4), is valid for materials

showing a strain/energy transformed into heat dependency as alloy Al 6082 in
*this experiment. The temperature increase ∆T , measured during the tests at*
*room temperature T*0 *= 296 K, and for a plastic-strain value εp* *= 0.027, can*
*be determined from Table 2, these values being ∆T = 3 K for ˙εp* = 600 s*−1*
*and ∆T = 3.2 K (extrapolated from εp* _{= 0.026) for ˙ε}p_{= 1000 s}*−1*_{. Both}
temperature-increase values are practically equal, and thus it can be deduced
*that the proportion of plastic work converted into heat β does not depend on*
the strain rate for alloy Al 6082.

Nevertheless, no conclusions can be drawn with respect to the dependency
*of β on temperature because the mechanical behaviour of alloy Al 6082 *
*de-pends heavily on temperature. The variation of the temperature increase ∆T*
associated with plastic strain is due to mainly the aforementioned dependency.

These results lead to the conclusion that the use of the Zehnder model is appropriate in this case, since the tested material is not strain-rate dependent as reported before.

The temporal evolution of the stress-strain state of the system was analysed
by direct integration of the equations of motion and the constitutive equations.
The implicit algorithm proposed by Zaera and Fern´andez-S´aez (2006) was
used to integrate the Johnson-Cook constitutive equation. This algorithm was
*modiﬁed to include the dependency of β on εp*_{, Eq. (1.4).}

For the validation of the numerical model proposed, the experimental and the analytical elastic waves were compared. Figure 9 shows the experimental and numerical incident, reﬂected and transmitted nominal stress waves; the three waves verify the relation

*εI+ εR= εT* (3.3)

A good agreement between the experiments and numerical results was found. The radial-nominal stress component is also plotted in Fig. 9. It can be seen that the values of this wave are practically negligible, allowing for the fulﬁlment of the hypothesis of negligible radial inertia during the SHPB test due to the initial shape geometry (Malinowski and Klepaczko, 1986).

*3.3.2.* *Results*

*Figure 10 shows the relations σ−εp*_{found during the numerical analyses at}
room temperature and a strain rate of 300 s*−1*_{, 600 s}*−1*_{, and 1000 s}*−1*_{, together}
*with the β − εp* _{relations calculated using Eq. (1.4). It may be observed that}
*the usual hypothesis taking β as constant is, in this case, available for high*
*plastic-strain values. The medium value calculated for β was 0.9, which is*
similar to that currently used for metal alloys.

Fig. 9. Incident, reﬂected and transmitted longitudinal-nominal stress waves and radial-nominal stress wave

*Fig. 10. Relations σ − εp* _{and β − ε}p_{for diﬀerent dynamic strain rates at room}

temperature

Figures 11a and 11b show, respectively, a map of the plastic deformation
*and the temperature increase for calculation time of t = 120 µs, initial *
*tem-perature of 296 K and a strain rate of ˙εp* = 1000 s*−1*_{.}

The cylindrical surface of the specimen shows uniform ﬁelds of plastic de-formation (Fig. 11a and temperature Fig. 11b). It is observed using numerical simulations that on the specimen bases, local increaments of plastic defor-mation and temperature take place as observed during experiments using IR temperature measurements. These local increaments are related to friction ef-fects between the specimen and the bars. Localized small non-symmetrical irregularities are also noticed; these irregularities are due to the non-exact cylindrical symmetry of the mesh. A temperature increase on the specimen

Fig. 11. (a) Plastic strain and (b) temperature maps resulting from numerical
*simulation at room temperature for a strain rate ˙εp*

= 1000 s*−1*and corresponding

*to a plastic strain value εp _{= 0.07}*

surface (initial test temperature equal to 296 K) between 7 K and 13 K can be seen. This value is of the same order as the one measured during the experi-ments (Table 2).

Figure 12 gives the numerical (continuous line) and experimental (symbol) temperature proﬁles along a generatrix line taken on the surface of the de-formed specimen. The numerical proﬁle corresponds to the temperature map using Fig, 11b. The two proﬁles discussed above show a good agreement. The temperature increase at the contact between the bars and specimen was higher than the temperature increase in the specimen middle zone, due to friction ef-fects. The diﬀerence in the central zone is due to a possible variation of the soot coating due to its ejection during experiments.

Fig. 12. Experimental and numerical temperature proﬁles for an imposed strain level
*under dynamic compression and corresponding to a strain level of εp _{= 0.07}*

As a result of numerical simulations, the temperature increments of the
specimen surface were calculated and compared with the experimental results.
Figure 13 shows the temperature evolution during the plastic-deformation
pro-cess for two diﬀerent strain rates using numerical simulations. The simulated
*tests were at ˙εp* = 600 s*−1* _{and ˙ε}p_{= 1000 s}*−1*_{, both at room }
*temperatu-re, and at 373 K and ˙εp* = 1500 s*−1*_{. Figure 13 also plots the experimental}
temperature-increase values associated with the corresponding plastic-strain
values (Table 2).

*Fig. 13. Numerical and experimental T − εp* _{results for diﬀerent strain rates under}

dynamic compression

A good agreement is observed between the experiments and numerical
*simulations in terms of the temperature increase ∆T for the strain-rates and*
test temperature considered.

**4.** **Conclusions**

By an experimental procedure developed, the temperature increase associated with plastic deformation during SHPB tests was measured for an Al alloy 6082. The results of the tests reveal that the temperature increases with the strain rate and decreases when the initial test temperature is higher.

At the ﬁnal deformation stage, a minor temperature decrease occurs, pre-sumably associated with an elastic unloading process.

A three-dimensional numerical model of the SHPB test including the in-cident bar, transmitter bar, the projectile and the specimen was developed.

The Zehnder model was linked to an implicit integration algorithm and im-plemented as a user subroutine in the commercial ﬁnite-elements code ABA-QUS/Explicit. This model oﬀers a prediction in terms of temperature increase associated with plastic deformation.

The results validated the applicability of Zehnder’s expression to model
*the proportion of plastic-deformation energy transformed into heat β for *
ma-terials that are strain dependent and strain rate non-dependent. Nevertheless,
*no conclusions could be drawn with respect to the dependency of β on *
tem-perature.

A good agreement was found between the experimental and numerical results, providing a better understanding of experimental measurement using an inverse method.

*Acknowledgements*

The author from UC3M thanks Dr. Rolando Guzm´an López for his collaboration, interest and discussions.

**References**

1. Agena A.S.M., 2009, A study of ﬂow characteristics of nanostructured
*Al-6082 alloy produced by ECAP under upsetting test, J. of Mater. Proc Tech.,*

**209, 2, 856-863**

2. Aravas N., Kim K.S., Leckie F.A., 1990, On the calculations of the stored
**energy of cold work, J. Eng. Mater. Technol., 112, 4, 465-470**

3. Chrysochoos A., Louche H., 2000, An infrared image processing to
* analy-se the caloriﬁc eﬀects accompanying strain localisation, Int. J. Eng. Sci., 38,*
1759-1788

4. Dadbakhsh S., Karimi Taheri A., Smith C.W., 2010, Strengthening study
on 6082 Al alloy after combination of aging treatment and ECAP process,
*Mater. Sci. and Eng.: A***, 527, 18/19, 4758-4766**

5. Guduru P.R., Rosakis A.J., Ravichandran G., 2001, Dynamic shear
*bands: an investigation using high speed optical and infrared diagnostics, *
*Me-chanics of Material***, 33, 371-402**

6. Guzm´an R., Essa Y.E., Mel´endez J., Aranda J., López F., P´
erez-Castellanos J.L., 2009, Measurement of temperature increment in
*compres-sive quasi-static and dynamic tests using the infrared thermography, Strain,*

7. Hodowany J., Ravichandran G., Rosakis A.J., Rosakis P., 1999,
*Par-tition of plastic work into heat and stored energy in metals, Experimental *
*Me-chanics***, 40, 113-123**

8. Jankowiak T., Rusinek A., Lodygowski T., 2011, Validation of the
Klepaczko-Malinowski model for friction correction and recommendations on
* split Hopkinson pressure bar, Finite Elements in Analysis and Design, 47, 10,*
1191-1208

9. Kappor R., Nemat-Nasser S., 1998, Determination of temperature rise
**du-ring high strain rate deformation, Mechanics of Material, 27, 1-12**

10. Karlsson and Sorensen, Inc., 2006, Abaqus, v6.4 User’s Manual

11. Klepaczko J.R., Rusinek A., Rodr´ıguez-Mart´ınez J.A., Pecherski
R.B, Arias A., 2009, Modeling of thermo-viscoplastic behaviour of DH-36
and Weldox 460-E structural steels at wide ranges of strain rates and
*tempera-tures, comparison of constitutive relations for impact problems, Mechanics of*
*Material***, 41, 599-621**

12. Kolsky H., 1949, An investigation of the mechanical properties of materials
**at very high rates of loading, Proc. Phys. Soc., B62, 676-699**

13. Macdougall D., Harding J., 1998, The measurement of specimen surface
*temperature in high-speed tension and torsion test, Int. J. of Impact Engin.,*

**21, 6, 473-488**

14. Malinowski J.Z., Klepaczko J.R., 1986, A uniﬁed analytic and numerical
*approach to specimen behaviour in the Split-Hopkinson pressure bar, Int. J.*
*Mech. Sci.***, 28, 6, 381-391**

15. Mann T., H¨arkeg˚ard G., St¨ark K., 2007, Short fatigue crack growth in
**aluminium alloy 6082-T6, Int. J. of Fatigue, 29, 8/11, 1820-1826**

16. Manping L., Hans J.R., Yingda Y., Jens C.W., 2008, Deformation
struc-tures in 6082 aluminium alloy after severe plastic deformation by equal-channel
**angular pressing, Mater. Sci. and Eng., A, 483/484, 59-63**

17. Manson J.J., Rosakis A.J., Ravichandran, 1994, On the strain and strain
rate dependence of the fraction of plastic work converted to heat: an
*experimen-tal study using high speed infrared detectors and the Kolsky bar, Mechanics of*
*Material***, 17, 135-145**

18. Miguelez M.H., Zaera R., Molinari A., Cheriguene R., Rusinek A.,
2009, Residual stresses in orthogonal cutting of metals: The eﬀect of
*thermo-mechanical coupling parameters and of friction, Journal of Thermal Stresses,*

**32, 269-289**

19. Mrówka-Nowotnik G., Sieniawski J., 2005, Inﬂuence of heat treatment
on the microstructure and mechanical properties of 6005 and 6082 aluminium
**alloys, J. of Mater. Proc. Tech., 162/163, 367-372**

20. Oussouaddi O., Klepaczko J.R., 1991, An analysis of transition from
*iso-thermal to adiabatic deformation in the case of a tube under torsion, *
*Proce-edings of the conference on DYMAT 91. J. Phys. IV*; Coll. C3 (Suppl. III):
C3-C323

21. P´erez-Castellanos J.L., Guzm´an R., Rusinek A., Mel´endez J., 2010,
Temperature increment during quasi-static compression tests using Mg metallic
**alloys, Materials and Design, 31, 7, 3259-3269**

22. Rabin Y., Rittel, D., 2000, Infrared temperature sensing of mechanically
* loaded specimens: thermal analysis, Experimental Mechanics, 40, 197-202*
23. Rodr´ıguez-Mart´ınez J.A., Rusinek A., Chevrier P., Bernier R.,

Arias A., 2010, Temperature measurements on ES steel sheets subjected to
* perforation by hemispherical projectiles, Int. J. Impact. Eng., 37, 828-841*
24. Rosakis P., Rosakis A.J., Ravichandran G., Hodowany J., 2000, A

thermodynamic internal variable model for the partition of plastic work into
* heat and stored energy in metals, Journal Mech. Phys. Solids, 48, 581-607*
25. Rusinek A., Klepaczko J.R., 2001, Eﬀect of adiabatic heating in some

*pro-cesses of plastic deformation, 4th International Symposium on Impact *
*Engine-ering*, Kunamoto, Jap´* an, Impact Engineering and Application, I/II, 37-53*
26. Rusinek A., Nowacki W.K., Gadaj P., Klepaczko J.R., 2003,

Measure-ment of temperature coupling by thermovision and constitutive relation at high
* strain rates for the dual phase sheet steel, Journal de Physique IV France, 110,*
411-416

27. Rusinek A., Klepaczko J.R., 2007, Experiments on heat generated during
*plastic deformation and stored energy for TRIP steels, Materials and Design,*

**30, 35-48**

28. Rusinek A., Zaera R., Klepaczko J.R., 2007, Constitutive relations in 3-D
for a wide range of strain rates and temperatures – application to mild steels,
*Int. J Solids Structures***, 44, 5611-5634**

29. Rusinek A., Cheriguene R., Baumer A., Klepaczko J.R., Larour P.,
2008, Dynamic behaviour of high-strength sheet steel in dynamic tension,
*expe-rimental and numerical analyses, Journal of Strain Analysis for Engineering*
*Design***, 43, 37-53**

30. Taylor G.I., Quinney M.A., 1934, The latent energy remaining in a metal
**after cold working, Proc. R. Soc. London, A143, 307-326**

*31. Thomson W. (Lord Kelvin), 1853, On dynamical theory of heat, Trans. R.*
*Soc. Edimb.*, 261-282

32. Trojanowski A., Macdougall D., Harding J., 1998, An improved
techni-que for the experimental measurement of specimen surface temperature during
**Hopkinson-bar tests, Measurement Sci. Tech., 9, 12-19**

33. Zaera R., Fern´andez-S´aez J., 2006, An implicit consistent algorithm for the
integration of thermoviscoplastic constitutive equations in adiabatic conditions
* and ﬁnite deformations, International Journal of Solids and Structures, 43, 6,*
1594-1612

*34. Zehnder A.T., 1991, A model for the heating due to plastic work, Mechanics*
*Research Communications***, 18, 1, 23-28**

**Wzrost temperatury wywołany plastycznym odkształceniem przy**
**dynamicznym ściskaniu – analiza stopu aluminium Al 6082**

Streszczenie

Wzrost temperatury w materiale związany z plastycznym odkształcaniem może być rejestrowany różnymi metodami, w tym m.in. techniką termograﬁi podczerwie-ni (IRT). Prezentowana praca poświęcona jest badapodczerwie-niom wzrostu temperatury przy różnym tempie odkształceń i temperatury początkowej próbek wykonanych ze stopu aluminium Al 6082. W eksperymentach użyto zmodyﬁkowanego pręta Hopkinsona do generowania szybko-zmiennych odkształceń w materiale i jednocześnie dokonywa-no pomiarów temperatury za pomocą kamery termowizyjnej. Przeprowadzodokonywa-no także symulacje numeryczne przebiegu przyrostu temperatury pozwalające na lepsze zro-zumienie zachodzących procesów na podstawie lokalnych pomiarowym. W tym celu zbudowano szczegółowy model bazujący na metodzie elementów skończonych, któ-ry przeanalizowano pod kątem dynamicznego ściskania. Część pracy odkształcenia plastycznego zamienianego w ciepło oszacowano za pomocą modelu Zehndera. Wy-niki obliczeń uwzględniających tempo odkształceń i temperaturę początkową na jej przyrost w badanym materiale zweryﬁkowano z rezultatami doświadczeń.